* Your assessment is very important for improving the work of artificial intelligence, which forms the content of this project
Materials Transactions, Vol. 45, No. 10 (2004) pp. 3028 to 3032 #2004 The Japan Institute of Metals Comparison among Mechanical Properties of Investment-Cast c.p. Ti, Ti-6Al-7Nb and Ti-15Mo-1Bi Alloys Chia-Wei Lin*1 , Chien-Ping Ju and Jiin-Huey Chern Lin*2 Department of Materials Science and Engineering, National Cheng-Kung University, 70101 Tainan Taiwan, R.O. China The present study compares castability and mechanical performance among alloys of c.p. Ti, Ti-6Al-7Nb and a newly-developed Ti-15Mo-1Bi in regard to their as-cast state. Experimental results indicate that average cast length of Ti-6Al-7Nb appears a little lower than c.p. Ti and Ti-15Mo-1Bi, although the diﬀerences are not signiﬁcant. C.p. Ti has an hcp phase of lath-type morphology with serrated, irregular grain boundaries. Ti-6Al-7Nb is dominated by hexagonal 0 phase with acicular martensitic morphology. In particular, Ti-15Mo-1Bi is comprised of equiaxed, metastable bcc phase. The hardened layer thicknesses of three materials are similar. Ti-15Mo-1Bi has the highest surface microvickers hardness, while c.p. Ti has the lowest. The bulk hardness of c.p. Ti is much lower than the other two alloys which display similar hardness. Notably, Ti-15Mo-1Bi and Ti-6Al-7Nb have similar bending strength which is far higher than c.p. Ti. The bending modulus of Ti-15Mo-1Bi is signiﬁcantly lower than c.p. Ti and Ti-6Al-7Nb. Ti-15Mo-1Bi also shows a much larger elastic recovery angle than two other materials. Tensile test indicates that Ti-15Mo-1Bi has a similar UTS but much higher YS and elongation along with much lower tensile modulus compared to Ti-6Al-7Nb. (Received June 15, 2004; Accepted August 2, 2004) Keywords: titanium alloy, investment casting, microstructure, mechanical properties 1. Introduction Commercially pure titanium (c.p. Ti) has established a reputation of low density, high corrosion resistance and excellent biocompatibility for dental prosthetic applications including crown and bridge, partial framework, dental implant, etc.1–3) Though titanium is highly reactive with both oxygen and molding materials at high temperatures, further developments in casting machines and molding materials have been proven to be capable of assuring the clinical use of titanium dental castings.4–6) Despite its many good properties, some disadvantages (especially relatively low strength) of cast pure titanium have often been criticized to be insuﬃcient for certain dental applications such as long-spanned ﬁxed prostheses and the frameworks of removable partial dentures (RPD).4,7–10) Ti6Al-7Nb alloy was originally developed using niobium to replace vanadium in Ti-6Al-4V for orthopedic applications.11) Then, this alloy has also been used as a dental casting metal, especially in Japan. Kobayashi et al.12) showed that Ti-6Al-7Nb alloy exhibited suﬃcient castability, suitable mechanical properties and excellent corrosion resistance for dental application. At this writing, Ti-15Mo alloy has come to be known as having a bcc structure with a good combination of strength, modulus and elongation.13) Also, the addition of bismuth was reported to be very eﬀective in lowering the surface tension (surface energy) of molten titanium and improving castability.14) This work compares castability and mechanical performance among c.p. Ti, Ti-6Al-7Nb and our newly-developed Ti-15Mo-1Bi alloy in terms of their as-cast state. Speciﬁcally, the microstructure, phase constituents, bending and tensile behavior, along with castability of the three materials are investigated and compared. *1Graduate Student, National Cheng-Kung University author, E-mail: [email protected], National ChengKung University *2Corresponding 2. Experimental Methods The materials used for this study are to be characterized as c.p. Ti, Ti-6Al-7Nb and Ti-15Mo-1Bi alloys (Note: all compositions in this study are presented by weight). All materials were prepared from raw materials including titanium (99.8% in purity), molybdenum (99.95% in purity), niobium (99.8% in purity), aluminum (99.95% in purity) and bismuth (99.5% in purity) using a commercial arc-melting vacuum-pressure type casting system (Castmatic, Iwatani Corp., Japan). Prior to melting/casting, the melting chamber was evacuated and purged with argon. An argon pressure of 1.5 Pa was maintained during melting. Appropriate amounts of various metals were melted in a U-shaped copper hearth with a tungsten electrode. The ingot was turned upside-down and re-melted three times to improve chemical homogeneity. Just before casting, the ingot was melted again in an openbased copper hearth under an argon pressure of 1.5 Pa. The diﬀerence in pressure between the two chambers allowed the molten alloy to instantly drop into a mold composed of magnesia-based investment material heated to 473 K. A scanning electron microscopy (SEM)-energy dispersive spectroscopy (EDS) analysis indicates that chemical compositions of two cast alloys (Ti-5.9Al-7.0Nb and Ti-14.9Mo1.2Bi, respectively) were quite close to those designed. To serve various purposes for this study, three diﬀerent kinds of wax patterns were used for casting, i.e., (1) six needle-shaped patterns, 0.45 mm dia. nylon lines (Fig. 1) for the evaluation of castability; (2) slab-shaped (36 mm 5 mm 1:5 mm) patterns for metallographic examination, X-ray diﬀraction (XRD), three-point bending and hardness tests; and (3) patterns for tensile test with a gage length of 10 mm and rectangular cross section of 3 mm 1:5 mm. Castability of these diﬀerent materials was evaluated by their cast lengths. As for data analysis one-way ANOVA followed by Student-Newman-Kuels test was used to evaluate statistical signiﬁcance of the data. In all cases the statistical diﬀerences were considered signiﬁcant at p < 0.05. Comparison among Mechanical Properties of Investment-Cast c.p. Ti, Ti-6Al-7Nb and Ti-15Mo-1Bi Alloys 3029 Table 1 Cast lengths of investigated materials. Material Cast length (mm) c.p. Ti 27:0 4:9 Ti-6Al-7Nb Ti-15Mo-1Bi 25:7 2:9 28:4 4:1 vickers hardness tester with a load of 0.2 kg for 15 seconds. To determine the variation in hardness with sample depth, the microvickers hardness tests were performed on the crosssections of castings. 3. Fig. 1 Speciﬁcation of nylon pattern used for castability evaluation. XRD for phase analysis was conducted using a Rigaku diﬀractometer (Rigaku D-max IIIV, Rigaku Co., Tokyo, Japan) operated at 30 kV and 20 mA with a scanning speed of 1 /min. A Ni-ﬁltered CuK radiation was used for the study. A silicon standard was used for calibrating diﬀraction angles with various phases being identiﬁed by matching each characteristic peak in the diﬀraction patterns using JCPDS ﬁles. Surfaces of the cast alloys for microstructural study were mechanically polished via a standard metallographic procedure to a ﬁnal level of 0.05 mm alumina powder, followed by etching in a Kroll’s reagent comprising water, nitric acid, and hydroﬂuoric acid (80:15:5 in volume). Microstructure of the etched alloys was examined using an optical microscope (Leitz Labrorlux 12 Pols, Leica Co., Germany). Three-point bending tests were performed using a desk-top mechanical tester (Shimadzu AGS-500D, Tokyo, Japan) operated at a crosshead speed of 0.5 mm/s. The bending strength was determined using the equation, ¼ 3PL=2bh2 ,15) where is the bending strength (MPa); P is the load (kg), L is the span length (mm), b is the specimen width (mm), and h is the specimen thickness (mm). The modulus of elasticity in bending was calculated from the load increment and corresponding deﬂection increment between the two points on a straight line as far apart as possible using the equation, E ¼ L3 P=4bh3 , where E is the modulus of elasticity in bending (Pa), P is the load increment measured from preload (N), and is the deﬂection increment at midspan measured from preload. The average bending strength and modulus of elasticity were taken from ﬁve tests under each condition. The elastic recovery (springback) capability for each material was evaluated based on the changes in deﬂection angle when loading was removed. A servo-hydraulic type testing machine (EHF-EG, Shimadzu Co., Tokyo, Japan) was used for tensile test. Tensile testing was performed at room temperature at a constant crosshead speed of 8:33 106 m/s. Average ultimate tensile strength (UTS), yield strength (YS) at 0.2% oﬀset, modulus of elasticity and elongation to failure were taken from ﬁve tests under each condition. Hardness of the samples was evaluated using a Matsuzawa MXT70 micro- Results and Discussion Cast lengths (a measure of castability) of c.p. Ti, Ti-6Al7Nb and Ti-15Mo-1Bi are compared in Table 1. As indicated in the table, the average cast length of Ti-6Al-7Nb (25.7 mm) appears a little lower than those of c.p. Ti (27.0 mm) and Ti15Mo-1Bi (28.4 mm), despite the fact that the diﬀerences are not signiﬁcant. The little diﬀerence in ‘‘mold-ﬁlling index’’ (a measure of castability) between pure Ti and Ti-6Al-7Nb alloy was also indicated by Shimizu et al.16) Many factors have been considered to aﬀect the castability of a metal including mold design, mold temperature, cooling rate, molten metal temperature, surface tension, mold reaction, dendrite formation, etc.17) Since all process parameters (power level, heating duration, mold size, shape and temperature, etc.) were ﬁxed in the study, the factors that aﬀect castability most likely were material-related factors such as mold reaction, surface tension and dendrite formation. Ragone et al.18) indicated that the addition of an alloy element to a pure metal always lowers the ﬂuidity (increasing viscosity) of the metal due to the formation of dendrites that causes resistance to proceed ﬂuid ﬂow in the early stage of solidiﬁcation. From this point of view, the dendrite factor could not be ﬁtted in to explain the high castability of the proposed Ti-15 Mo-1Bi alloy. Rather, in an earlier study, Cheng et al.14) showed that the addition of bismuth could lower the surface tension (surface energy) of titanium and signiﬁcantly improve castability. The present study suggests that surface tension reduction caused by Bi-inducement may have a dominant eﬀect in maintaining high castability of the alloy. Titanium alloys may be categorized into diﬀerent types according to their room temperature phases.19) In this research work, aluminum is an -stabilizer, while molybdenum and niobium are intended as -isomorphous stabilizers. According to the binary Ti-Bi phase diagram, Bi is a eutectoid element. The XRD patterns and morphologies of three investigated materials are shown in Figs. 2 and 3, respectively. It can be seen that the as-cast c.p. Ti has an phase with hcp crystal structure. Figure 3(a) shows that this c.p. Ti has lath-type morphology with serrated, irregular grain boundaries, indicating a rapid cooling process during casting.13) The as-cast Ti-6Al-7Nb alloy was dominated by hexagonal 0 phase with a distorted hcp crystal structure.20) As shown in Fig. 3(b), Ti-6Al-7Nb has an acicular martensitic morphology with high-temperature -phase grain boundaries barely 3030 C.-W. Lin, C.-P. Ju and J.-H. C. Lin Fig. 4 Fig. 2 XRD patterns of investigated materials. visible. This acicular martensitic morphology is similar to that observed by Ahmed and Rack, who claimed that a high cooling rate is required for Ti-6Al-4V to attain a martensitic morphology.20) According to Filip et al.,21) a completely martensitic structure could be obtained at a cooling rate >18 K/s. This suggests that the cooling rate for the proposed casting process should be at least as high as 18 K/s. The as-cast Ti-15Mo-1Bi alloy was comprised primarily of equiaxed, metastable phase with bcc crystal structure (Fig. 3(c)). The retention of phase at higher Mo contents is consistent with both the early result reported by Davis et al.22) and the more recent result of Bania.23) Bania reported that a minimum of 10 mass% Mo was needed in a Ti-Mo alloy to Fig. 3 Cross-sectional microvickers hardness of investigated materials. fully stabilize phase at room temperature. Variations in microvickers hardness with depth from the surfaces of castings are demonstrated in Fig. 4. As can be seen from the graph, Ti-15Mo-1Bi depicts the highest surface hardness, while c.p. Ti is the lowest. The hardened layer ( case) thickness appears to be roughly 100–150 mm for all three materials. Although the microvickers hardness values in the interior (bulk) of Ti-15Mo-1Bi and Ti-6Al-7Nb are similar (about 350 HV), the surface hardness of Ti-15Mo-1Bi is signiﬁcantly higher than that of Ti-6Al-7Nb probably due to their diﬀerent degrees in reaction with mold material. In addition, the bulk microvickers hardness of c.p. Ti is much lower (about 200 HV). The hardened layer, that is almost unavoidable in investment-cast Ti and Ti-alloys, forms through the decomposition of the investment oxides and diﬀusion of the resulting elements into the casting.24,25) Although the measurements were straightforward, the interpretation of the data are complex. Such eﬀects as solution and/or precipitation hardening, grain size and crystal structure/phase would all aﬀect the hardness of the alloy. The primary cause to the relatively high surface hardness of Ti-15Mo-1Bi might be its stronger reaction with investment material during casting. A much higher bulk hardness level of Ti-15Mo-1Bi and Ti-6Al-7Nb (than c.p. Ti) is probably due Optical micrographs of investigated materials. Comparison among Mechanical Properties of Investment-Cast c.p. Ti, Ti-6Al-7Nb and Ti-15Mo-1Bi Alloys Material Table 2 Bending test data of investigated materials. Bending strength (MPa) Bending modulus (GPa) 3031 Elastic recovery angle (degree) c.p. Ti 925 21 104 4 7:7 0:2 Ti-6Al-7Nb 1943 26 111 3 22:0 0:4 Ti-15Mo-1Bi 1975 38 90 1 27:3 1:2 Table 3 Tensile test data of investigated materials. Material Yielding strength (MPa) Tensile strength (MPa) Tensile modulus (GPa) Elongation (%) c.p. Ti 429 20 544 21 105 8 18:0 1:8 Ti-6Al-7Nb Ti-15Mo-1Bi 824 18 953 34 1045 17 1013 29 126 8 98 5 3:7 0:8 7:8 2:1 to a combined eﬀect of solution hardening and their much ﬁner morphology. Bending properties of three cast materials are listed in Table 2. As indicated in the table, cast Ti-15Mo-1Bi and Ti6Al-7Nb alloys have similar bending strengths (1975 and 1943 MPa, respectively), which were far higher than that of cast c.p. Ti (925 MPa). The bending modulus of Ti-15Mo1Bi (90 GPa), however, is signiﬁcantly lower than those of Ti-6Al-7Nb (111 GPa) and c.p. Ti (105 GPa). One way ANOVA statistical analysis indicated that the diﬀerences are signiﬁcant. Kobayashi et al.12) suggested that the greater strength of Ti-6Al-7Nb alloy than c.p. Ti was due to a combined eﬀect of solution strengthening and structurereﬁning strengthening. Same eﬀect is suggested to account for the higher strengths of the proposed Ti-15Mo-1Bi and Ti6Al-7Nb alloys as compared with c.p. Ti. The lower bending modulus of Ti-15Mo-1Bi as opposed to the other two materials arising from a direct result of the presence of phase in the alloy.13) The relatively high strength and low modulus of Ti-15Mo1Bi lead to an elastic recovery angle which are larger than Ti6Al-7Nb by almost one-quarter and larger than c.p. Ti by as much as 2.5 times. High elastic recovery capability is an indication of high strength and low modulus and is essential for many load-bearing implant and dental applications. It is also worth noting that during bending all Ti-15Mo-1Bi and c.p. Ti samples had reached the pre-set deﬂection limit of 8 mm without failure. However, about 40% of all Ti-6Al-7Nb samples failed prior to reaching the pre-set limit, indicating a lower ductility level of the material. The lower ductility of Ti-6Al-7Nb than c.p. Ti and Ti-15Mo was also observed by Niinomi.26) The favorable mechanical performance of Ti-15Mo-1Bi was again conﬁrmed in tensile tests. As indicated in Table 3, Ti-15Mo-1Bi and Ti-6Al-7Nb alloys have far higher strengths and lower elongations than c.p. Ti. Comparison between the two alloys indicates that Ti-15Mo-1Bi has a similar UTS (1013 MPa) but much higher YS (953 MPa) and much lower tensile modulus (98 GPa) than those of Ti-Al7Nb (1045 MPa, 824 MPa and 126 GPa, respectively). This much larger elongation of Ti-15Mo-1Bi (7.8%) than Ti-6Al7Nb (3.7%) again displays the better ductility of Ti-15Mo1Bi. For a material to be used as a medical implant, an increase in material strength yet maintaining a low modulus is advantageous, since a low modulus material is generally favored for implant application for its reduced stressshielding eﬀect.27) From this point of view, Ti-15Mo-1Bi demonstrates a greater potential than the other two materials. Even with a large elongation value, the elastic recovery angle of c.p. Ti is still much lower than the other two materials due to its low strength. Practically, a larger elastic recovery angle means an increased adjustability without fear of breakage for a device (e.g., clasp for RPD). The higher ductility and the elastic recovery angle of Ti-15Mo-1Bi also indicate its superiority to the other two materials. 4. Conclusions The castability, bending and tensile properties of c.p. Ti, Ti-6Al-7Nb and Ti-15Mo-1Bi alloys were investigated. Obtained results are as follows. (1) The average cast length of Ti-6Al-7Nb is a little bit lower than that of c.p. Ti and Ti-15Mo-1Bi, although the diﬀerences are not signiﬁcant. (2) C.p. Ti has a hcp phase of lath-type morphology with serrated, irregular grain boundaries. Ti-6Al-7Nb was dominated by hexagonal 0 phase with acicular martensitic morphology. Ti-15Mo-1Bi was comprised of equiaxed, metastable bcc phase. (3) The hardened layer ( case) thicknesses of three materials were similar. Ti-15Mo-1Bi had the highest surface microvickers hardness, while c.p. Ti was the lowest. The bulk hardness of c.p. Ti was much lower than the other two alloys that had similar hardness. (4) Ti-15Mo-1Bi and Ti-6Al-7Nb had similar bending strengths which are far higher than c.p. Ti. The bending modulus of Ti-15Mo-1Bi was signiﬁcantly lower than c.p. Ti and Ti-6Al-7Nb. Ti-15Mo-1Bi showed a much larger elastic recovery angle than the other two materials. (5) Ti-15Mo-1Bi has a similar UTS but having much higher YS and elongation as well as much lower tensile modulus than Ti-Al-7Nb. 3032 C.-W. Lin, C.-P. Ju and J.-H. C. Lin REFERENCES 1) E. P. Lautenschlager and P. Monaghan: Int. Dent. J. 43 (1993) 245– 253. 2) H. Nakajima and T. Okabe: Dent. Mater. J. 15 (1996) 77–90. 3) M. Koike and H. Fujii: Biomaterials 22 (2001) 2931–2936. 4) T. Okabe and H. Herø: Cell. Mater. 5 (1995) 211–230. 5) K. Ida, T. Togaya, S. Tsutsumi and M. Takeuchi: Dent. Mater. J. 1 (1982) 8–21. 6) H. Hamanaka, H. Doi, T. Yoneyama and O. Okuno: J. Dent. Res. 68 (1989) 1529–1533. 7) T. Kawazoe and K. Suese: J. Dent. Med. 30 (1989) 317–328. 8) A. Kuroiwa and Y. Igarashi: J. Jpn. Prosthodont Soc. 42 (1998) 547– 558. 9) K. Watanabe, O. Miyakawa, Y. Takada, O. Okuno and T. Okabe: Biomaterials 24 (2003) 1737–1743. 10) J. Zhu, A. Kamiya, T. Yamada, W. Shi and K. Naganuma: Mater. Sci. Eng. A339 (2003) 53–62. 11) M. Semlitsch, F. Stabu and H. Weber: Biomed. Tech. 30 (1985) 334– 339. 12) E. Kobayashi, T. J. Wang, H. Doi, T. Yoneyama and H. Hamanaka: J. Mater. Sci. Mater. Med. 9 (1998) 567–574. 13) W. F. Ho, C. P. Ju and J. H. Chern Lin: Biomaterials 20 (1999) 2115– 2122. 14) W. W. Cheng, J. H. Chern Lin and C. P. Ju: AFS. Trans. 01-169 (2001) 987–996. 15) A. Guha: Metals Handbook, 9th ed., 8 (ASM International, Metals Park, OH, 1985) pp. 133. 16) H. Shimizu, T. Habu, Y. Takada, K. Watanabe, O. Okuno and T. Okabe: Biomaterials 23 (2002) 2275–2281. 17) L. F. Porter and P. C. Rosenthal: AFS Trans. 60 (1952) 725–739. 18) D. V. Ragone, C. M. Adams and H. F. Taylor: AFS Trans. 64 (1956) 640–653. 19) E. W. Collings: The physical metallurgy of titanium alloys, (ASM International, Metals Park, OH, 1984) pp. 5–11. 20) T. Ahmed and H. J. Rack: Mater. Sci. Eng. A243 (1998) 206–211. 21) R. Filip, K. Kubiak, W. Ziaja, J. Sieniawski: J. Mater. Process. Technol. 133 (2003) 84–89. 22) R. Davis, H. M. Flower and D. R. F. West: J. Mater. Sci. 14 (1979) 712– 722. 23) P. J. Bania: Beta titanium alloys in the 1990’s, ed. by D. Eylon, R. R. Boyer and D. A. Koss, (TMS, Warrendale, PA, 1993) pp. 3–14. 24) M. Kikuchi, Y. Takada, S. Kiyosue, M. Yoda, M. Woldu, Z. Cai, O. Okuno and T. Okabe: Dent. Mater. 19 (2003) 174–181. 25) O. Miyakawa, K. Watanabe, S. Okawa, S. Nakano, M. Kobayashi and N. Shiokawa: Dent. Mater. J. 8 (1989) 175–185. 26) M. Niinomi: Mater. Sci. Eng. A243 (1998) 231–236. 27) D. R. Sumner and J. O. Galante: Clin. Orthop. Relat. Res. 274 (1992) 202–212.